Rational Design of Ceramic-Like Molecular Ferroelectric by Quasi-Spherical Theory.
Wei, Zhen-Hong; Jiang, Zhen-Tao; Zhang, Xiu-Xiu; Li, Ming-Li; Tang, Yuan-Yuan; Chen, Xiao-Gang; Cai, Hu; Xiong, Ren-Gen; Journal of the American Chemical Society 142 (2020) 1995–2000; doi:10.1021/jacs.9b11665

data_4134100
_publ_section_title
;
 Rational Design of Ceramic-Like Molecular Ferroelectric by
 Quasi-Spherical Theory.
;
_journal_issue                   4
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              1995
_journal_page_last               2000
_journal_paper_doi               10.1021/jacs.9b11665
_journal_volume                  142
_journal_year                    2020
_chemical_formula_moiety         'C6 H13 N2, B F4'
_chemical_formula_sum            'C6 H13 B F4 N2'
_chemical_formula_weight         199.99
_space_group_crystal_system      orthorhombic
_space_group_IT_number           29
_space_group_name_Hall           'P 2c -2ac'
_space_group_name_H-M_alt        'P c a 21'
_atom_sites_solution_hydrogens   difmap
_audit_creation_method           SHELXL-2014/7
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   13.1375(9)
_cell_length_b                   7.6331(5)
_cell_length_c                   17.7668(11)
_cell_measurement_reflns_used    3067
_cell_measurement_temperature    173(2)
_cell_measurement_theta_max      30.3520
_cell_measurement_theta_min      2.6520
_cell_volume                     1781.7(2)
_computing_cell_refinement       'CrysAlisPro 1.171.39.46 (Rigaku OD, 2018)'
_computing_data_collection       'CrysAlisPro 1.171.39.46 (Rigaku OD, 2018)'
_computing_data_reduction        'CrysAlisPro 1.171.39.46 (Rigaku OD, 2018)'
_computing_molecular_graphics    'DIAMOND (Brandenburg & Putz, 2005)'
_computing_publication_material  'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_structure_solution    'SHELXL-2014/7 (Sheldrick, 2014)'
_diffrn_ambient_temperature      173(2)
_diffrn_measured_fraction_theta_full 0.998
_diffrn_measured_fraction_theta_max 0.998
_diffrn_measurement_device_type  'XtaLAB Synergy R, DW system, HyPix'
_diffrn_measurement_method       'four-circle diffractometer'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.1348
_diffrn_reflns_av_unetI/netI     0.1099
_diffrn_reflns_Laue_measured_fraction_full 0.998
_diffrn_reflns_Laue_measured_fraction_max 0.998
_diffrn_reflns_limit_h_max       13
_diffrn_reflns_limit_h_min       -15
_diffrn_reflns_limit_k_max       9
_diffrn_reflns_limit_k_min       -8
_diffrn_reflns_limit_l_max       21
_diffrn_reflns_limit_l_min       -21
_diffrn_reflns_number            9006
_diffrn_reflns_point_group_measured_fraction_full 0.998
_diffrn_reflns_point_group_measured_fraction_max 0.998
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         25.249
_diffrn_reflns_theta_min         2.668
_diffrn_source                   'Rotating-anode X-ray tube'
_exptl_absorpt_coefficient_mu    0.148
_exptl_absorpt_correction_T_max  0.971
_exptl_absorpt_correction_T_min  0.969
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'CrysAlisPro 1.171.39.46 (Rigaku OD, 2018)'
_exptl_crystal_colour            Colourless
_exptl_crystal_density_diffrn    1.491
_exptl_crystal_description       Block
_exptl_crystal_F_000             832
_exptl_crystal_size_max          0.210
_exptl_crystal_size_mid          0.210
_exptl_crystal_size_min          0.200
_refine_diff_density_max         0.899
_refine_diff_density_min         -0.364
_refine_diff_density_rms         0.095
_refine_ls_abs_structure_details
;
 Refined as an inversion twin.
;
_refine_ls_abs_structure_Flack   1.1(15)
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.002
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     236
_refine_ls_number_reflns         3211
_refine_ls_number_restraints     7
_refine_ls_restrained_S_all      1.002
_refine_ls_R_factor_all          0.1151
_refine_ls_R_factor_gt           0.0985
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.2000P)^2^+1.5300P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.2697
_refine_ls_wR_factor_ref         0.2873
_reflns_Friedel_coverage         0.930
_reflns_Friedel_fraction_full    0.998
_reflns_Friedel_fraction_max     0.998
_reflns_number_gt                2422
_reflns_number_total             3211
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            ja9b11665_si_002.cif
_cod_data_source_block           Pca21
_cod_database_code               4134100
_shelx_shelxl_version_number     2014/7
_shelx_estimated_absorpt_t_min   0.970
_shelx_estimated_absorpt_t_max   0.971
_shelx_res_checksum              46860
_shelx_hkl_checksum              7666